UNIVERSITI TEKNIKAL MALAYSIA MELAKA
THE EXPERIMENTAL INVESTIGATION OF FATIGUE TEST
FOR SPOT WELDED STRUCTURAL JOINT
This report submitted in accordance with the requirement of the Universiti Teknikal Malaysia Melaka (UTeM) for the Bachelor Degree of Manufacturing Engineering
(Manufacturing Process) with Honours.
MUHAMMAD NABIL BIN MOHAMMED SUFIAN B071210502
910706 – 05 – 5437
UNIVERSITI TEKNIKAL MALAYSIA MELAKA
BORANG PENGESAHAN STATUS LAPORAN PROJEK SARJANA MUDA
TAJUK: The Experimental Investigation Of Fatigue Test For Spot Welded Structural
SESI PENGAJIAN: 2015/16 Semester 1
Saya Muhammad Nabil Bin Mohammed Sufian mengaku membenarkan Laporan
PSM ini disimpan di Perpustakaan Universiti Teknikal Malaysia Melaka (UTeM)
dengan syarat-syarat kegunaan seperti berikut:
1. Laporan PSM adalah hak milik Universiti Teknikal Malaysia Melaka dan penulis. 2. Perpustakaan Universiti Teknikal Malaysia Melaka dibenarkan membuat salinan
untuk tujuan pengajian sahaja dengan izin penulis.
3. Perpustakaan dibenarkan membuat salinan laporan PSM ini sebagai bahan pertukaran antara institusi pengajian tinggi.
4. **Sila tandakan ( )
(Mengandungi maklumat yang berdarjah keselamatan
atau kepentingan Malaysia sebagaimana yang termaktub
dalam AKTA RAHSIA RASMI 1972)
(Mengandungi maklumat TERHAD yang telah ditentukan
oleh organisasi/badan di mana penyelidikan dijalankan)
348 Jalan Teratai 4,
Taman Bunga Raya Bukit Beruang,
** Jika Laporan PSM ini SULIT atau TERHAD, sila lampirkan surat daripada pihak berkuasa/organisasi
berkenaan dengan menyatakan sekali sebab dan tempoh laporan PSM ini perlu dikelaskan sebagai
Rujukan Kami (Our Ref) :
PENGKELASAN LAPORAN PSM SEBAGAI SULIT/TERHAD LAPORAN PROJEK SARJANA MUDA TEKNOLOGI KEJURUTERAAN PEMBUATAN
(Manufacturing Proses)Muhammad Nabil Bin Mohammed Sufian
Sukacita dimaklumkan bahawa Laporan PSM yang tersebut di atas bertajuk
“The Experimental Investigation Of Fatigue Test For Spot Welded Structural Joint” mohon dikelaskan sebagai *SULIT / TERHAD untuk tempoh LIMA (5)
tahun dari tarikh surat ini.
2. Hal ini adalah kerana IANYA MERUPAKAN PROJEK YANG DITAJA OLEH SYARIKAT LUAR DAN HASIL KAJIANNYA ADALAH SULIT.
Sekian dimaklumkan. Terima kasih.
Tandatangan dan Cop Penyelia
* Potong yang tidak berkenaan
NOTA: BORANG INI HANYA DIISI JIKA DIKLASIFIKASIKAN SEBAGAI SULIT
I hereby, declared this report entitled The Experimental Investigation Of Fatigue Test For Spot Welded Structural Joint is the results of my own research except as cited in
This report is submitted to the Faculty of Engineering Technology of UTeM as a partial fulfillment of the requirements for the degree of Bachelor of Engineering Technology (Manufacturing Process) (Hons.). The member of the supervisory is as follow:
The experimental investigation of fatigue test for spot welded structural joint is a study about joining using the resistance spot welding and been testing using fatigue machine. This study more focuses on using of different type of material and different thickness that using aluminium and galvanized iron with thickness 1 mm and 0.5 mm each. The parameter for the resistance spot welding and fatigue machines is constant for each specimen used. The S-N curve is obtained from the fatigue testing for each specimen. The result shows that the combination of aluminium-galvanized iron with thickness 1 mm each is easy to fail and have low number of cycle. Furthermore, the aluminium thickness 1 mm and 0.5 mm joining shows that the specimen failures at number of cycle 58 with fatigue stress 2.71 MPa while for galvanized iron material fail at number of cycle 8409 with fatigue stress 2.28 MPa. It shows that the joining of galvanized iron material more strong than the aluminium material joining.
To my father & my mother,
Mr. Mohammed Sufian Bin Abdul Ghani & Mrs. Norridah Binti Rahim
All my friends and relatives
All the lecturers especially Mr. Mohammad Khalid Bin Wahid Thousand thank and appreciate for your support,
Bismillah ir-Rahman ir-Rahim,
Alhamdulilah thank to Allah the Most Gracious and Most Merciful for His grace and permission to finish my Final Year Project with successfully as required in fulfillment for my Bachelor’s in Engineering Technology (Manufacturing Process) from Universiti Teknikal Malaysia Melaka.
I would like to express my thanks to Mr. Mohammad Khalid Bin Wahid for his sincere advice and guidance provided throughout my studies. His patience, knowledge and trust personality have always been an inspiration for me and deeply influence my career and future life.
2.1 Material Properties... 6
2.2 Welding... 9
2.2.2 Application of Welding ... 9
2.2.3 Welding and Joining Processes ... 11
2.2.4 Safety in Welding ... 12
2.3 Resistance Spot Welding ... 14
2.3.1 Principle of the Resistance Spot Welding ... 14
2.3.2 Resistance Spot Welding Equipment ... 19
2.3.3 Resistance Spot Welding Parameter... 20
2.4 Fatigue Testing ... 25
2.4.1 Crack initiation (Ni) ... 26
2.4.2 Crack growth, Np ... 27
2.5 Fatigue Testing For Spot Welded Joint ... 29
CHAPTER 3 ... 31
METHODOLOGY ... 31
3.0 Introduction... 31
3.1 Flow chart ... 31
3.2 Prepare and Cutting Material ... 33
3.2.1 Prepare Material ... 33
3.2.2 Cutting Material ... 33
3.3 Joining Process ... 34
3.4 Testing ... 36
CHAPTER 4 ... 39
RESULT AND DISCUSSION ... 39
4.0 Collection of Result ... 39
4.1 Calculation Fatigue Stress ... 39
4.3 Result ... 41
4.4 Comparison the Specimen ... 56
4.4.1 Different Thickness ... 56
4.4.2 Comparison for different type of material ... 58
CHAPTER 5 ... 60
CONCLUSION AND RECOMMENDATION ... 60
5.0 Conclusion ... 60
5.1 Recommendation ... 61
APPENDIX ... 62
LIST OF FIGURES
Figure 1.1: Resistance Spot Welding Machine 2
Figure 1.2: Weld Nugget 3
Figure 1.3: Flow Chart 5
Figure 2.1: Space shuttle 10
Figure 2.2: Robot welding use in automobile industries 10
Figure 2.3: Welding Mask 13
Figure 2.4: Ventilation in Welding 13
Figure 2.5: Spot Welding Time Cycle 15
Figure 2.6: Lap joint 16
Figure 2.7: Work stages of resistance welding 17 Figure 2.8: Principle of Resistance Spot Welding 17 Figure 2.9: Schematic drawing of a resistance spot welding system 19
Figure 2.10: Ordinary Spot Welding Machine 20
Figure 2.11: Different phases of the fatigue life 26
Figure 2.12: Universal-tester 27
Figure 3.1: Flow Chart Method 32
Figure 3.2 : Size of fatigue test specimens 33
Figure 3.3: Foot Shearing Machine 34
Figure 3.4: Inventer AS-25 Resistance Spot Welding Machine 34
Figure 3.5: Mounting of specimen 35
Figure 3.6: Air servo Fatigue Testing Machine 36 Figure 3.7 : Mounting the specimen with the jig 37
Figure 3.8: Operation Flow Fatigue Testing 38
Figure 4.1: Shear Force 40
Figure 4.2: Graph of S-N curve aluminium thickness 0.5mm 42
Figure 4.3: Specimen after testing 43
Figure 4.4: Graph of S-N curve aluminium thickness 1mm 44
Figure 4.6: Graph of S-N curve galvanized iron thickness 0.5mm 46
Figure 4.7: Specimen after testing 47
Figure 4.8: Graph of S-N curve galvanized iron thickness 1mm 48
Figure 4.9: Specimen after testing 49
Figure 4.10: Graph of S-N curve aluminium thickness 1mm and 0.5mm 50
Figure 4.11: Specimen after testing 51
Figure 4.12: Graph of S-N curve galvanized iron thickness 1mm and 0.5mm 52
Figure 4.13: Specimen after testing 53
Figure 4.14: Graph of S-N curve aluminium and galvanized iron 1mm 54
LIST OF TABLE
Table 2.1: Welding Parameter 24 Table 3.1 : Resistance Spot Welding parameter 35 Table 4.1 Data for S-N curve aluminium thickness 0.5mm 42 Table 4.2: Data for S-N curve aluminium thickness 1mm 44 Table 4.3: Data for S-N curve galvanized iron with thickness 0.5mm 46 Table 4.4: Data for S-N curve galvanized iron Thickness 1mm 48 Table 4.5: Data for S-N curve aluminium thickness 1mm and 0.5mm 50 Table 4.6: Data for S-N curve galvanized iron thickness 1mm and 0.5mm 52 Table 4.7: Data for S-N curve aluminium and galvanized Iron 1mm 54
Table 4.8: Comparison result for aluminium 56
Spot welding is a broadly employed method to join sheet metals for body and cap structure in the automotive industry. The strength of the spot welds in the unibody vehicle structure decides the integrity of the structural performance during the vehicle operations. Most spot welds generally carry only shear forces however spot welds can likewise experience a significant amount of peel force or the force normal to the spot weld in certain stacking conditions. The mix of the stress states and geometric shapes of the spot welds lead to stress concentration that can bring in fatigue crack initiation around the spot weld. The presence of fatigue cracks can degrade structural performance and increase noise and vibration of the vehicle structure. Subsequently, comprehension of the fatigue strength for the spot welds is very critical in automotive component design. (Rahman M. , 2009)
The main motive of this project is to study about the fatigue testing of spot welding joint with using different type of material and different thickness of material. It is also want to know at what cycle the joint will be break using the fatigue testing machine and study the effect of using different type and thickness material.
Figure 1.1: Resistance Spot Welding Machine
1.1 Problem Statement
The problem in this experiment is to know the effect of spot welded joining using different type and thickness of material whether the joining is strong to support the load. This type of joining is important to be test because it has been using to assembly the component of the car. It is use in daily life of the human and involves the life.
Besides, other problem in this joining is to know the strength the spot welded joining with analyze the number of cycle using S-N curve. Each specimen will undergo fatigue testing and the result will be calculated using formula to plot the S-N curve. The S-N curve is “S” stands for stress and “N” stands for the number of cycle to failure.
Figure 1.2: Weld Nugget
The objectives of this project are:
i. To study the joining strength with different material and thickness from dynamic force
ii. To define the number of cycle using fatigue testing for spot welded joint
There are several scopes to be considered:
i. Type of joint
ii. Spot welding machine iii. Fatigue machine iv. Type of material
1.4 Flow Chart Planning
Figure 1.3: Flow Chart Start
Research Methodology Problem statement
Introduction Title Selection
Presentation PSM 1
End Presentation PSM 2 Discussion and Conclusion
One of the requirement task when conducting a research study is to gain understanding by reviewing the existing literature on the topic and use it in construction of own study. It is a tool to broaden our knowledge base in our research, focus to our research problem and bring clarity.
Meanwhile, previous study can improve our methodology and help us contextualize our findings. It is crucial in order to benchmarking our findings with others and add a body of knowledge thus developing a theoretical framework for our own study by following simple procedure where we search the literature in our area of interest and review the selected studies.
2.1 Material Properties
7 a) Aluminium
Aluminum is low density and therefore low weight, high strength, superior malleability, easy machining, excellent corrosion resistance and good thermal and electrical conductivity are amongst aluminum’s most important properties. Aluminum is also very easy to recycle.
Aluminum alloys commonly have tensile strengths of between 70 and 700 MPa. The range for alloys used in extrusion is 150 – 300 MPa. Unlike most steel grades, aluminum does not become brittle at low temperatures. Instead, its strength increases. At high temperatures, aluminum’s strength decreases. At temperatures continuously above 100°C, strength is affected to the extent that the weakening must be taken into account.
Features facilitating easy jointing are often incorporated into profile design. Fusion welding, Friction Stir Welding, bonding and taping are also used for joining.
iii. Corrosion resistance
8 b) Galvanized Iron
i. Strength and Ductility
The galvanizing process has no effect on the tensile, bend or impact properties of any of the structural steels investigated when these are galvanized in the “as manufactured” condition.
The occurrence of embrittlement depends on a combination of factors. Under certain conditions, some steels can lose their ductile properties and become embrittled. Several types of embrittlement may occur but of these only strain-ages embrittlement is aggravated by galvanizing and similar processes.
iii. Fatigue Strength
2.2.1 Welding Definition
Weld is defined by the American Welding Society (AWS) as a “localized coalescence (the combination or growing together of the grain structure of the materials being welded) of metals or non-metals method either by heating the materials to the required welding temperatures, with or without the utilization of pressure, or by the application of pressure alone, and with or without the use of filler materials”. In less technical language, a weld is made when separate pieces of material to be joined combine and form one piece when enough heat is applied to raise the temperature sufficiently enough to cause softening or dissolving and the pieces flow together enough pressure is used to force the pieces together so that the surfaces coalesce, enough heat and pressure are utilized together to force the different pieces of material to combine and form one piece. A filler material may or may not be added to the joint to form a completed weld joint.
2.2.2 Application of Welding